Tải bản đầy đủ - 0trang
3 SiO 2 -Insulated Metal Interconnects
26.3 SiO2 -Insulated Metal Interconnects
While still in the membrane, the SiO2 -coated pores can be electrochemically filled
with metal followed by membrane etching to give free-standing insulated wires
(Fig. 26.1, route 2; for details on synthesis and electrical measurements see ).
Typical TEM images (Fig. 26.2c, d) show the gold wires inside uniformly thick
and smooth silica tubes. The tube walls remain defect-free and no metal penetration
of the walls is seen. The top ends of the wires are typically flat or convex, unlike
nanowires grown in unmodified alumina membranes, which have cup-shaped ends.
This cup-like shape has been explained as a consequence of the high surface tension
of the alumina pore walls [23b]. The interaction of gold with the less polar silica
pores is apparently weaker. The coulombic efficiency for plating Au and Ni wires is
about 1.2 times higher (judging from wire lengths) in silica-modified pores than it
is in unmodified anodic alumina.
Fig. 26.4 Top: I−V characteristics of SiO2 -coated gold nanowires with different thickness of SiO2
(nm): (1) 25, (2) 14, (3) 8, (4) 4.5, (5) 3.5. A scheme of a test structure for measuring the electrical
properties is shown in the inset. Bottom: Optical micrograph of a test structure for measuring
the electrical properties of SiO2 -coated gold nanowires (left). A plot of the breakdown voltage
versus thickness (right). Reprinted with permission from . Copyright 2003 Wiley-VCH Verlag
GmbH & Co
Design and Assembly of High-Aspect-Ratio Silica-Encapsulated Nanostructures
When the silica-coated nanowires are released from the membrane, both ends
are open, because the tube-shells break near the ends of the metal wire (Fig. 26.2d).
This allows one to make electrical contact by evaporating metal onto the wire ends.
The I−V characteristics of SSG SiO2 films of different thicknesses (measured in
Au@SiO2 /Au configuration) are shown in Fig. 26.4 (top). The curves show typical
insulating behavior with breakdown voltages that increase linearly with film thickness (Fig. 26.4, bottom). The hard breakdown field is estimated at 4.8 MV cm–1 ,
which is only slightly less than the breakdown fields (10–15 MV cm–1 ) of the SiO2
dielectric used in CMOS integrated-circuit technology.
Because the SiO2 tubes are porous, their dielectric constant is expected to be
lower than that of dense silica (ε = 3.8 ). Porous silica is a promising dielectric material for nanoelectronics applications because of its relatively low dielectric
constant . Theoretical calculations predict a dielectric constant of 1.8–2.8 for
a volume pore fraction of 0.4 and an almost linear decrease in ε with increasing porosity. In our experiments, it was difficult to measure the dielectric constant
of the SiO2 films precisely because of the uncertainty in the contact area in the
Au@SiO2 /Au configuration. Nevertheless it is interesting to note that the synthesis offers some control over porosity, and that this will probably be reflected in the
dielectric constant of the films.
26.4 Coaxially Gated In-Wire Thin Film Transistors
On the way toward realization of nano- and molecular-scale electronics, the development of strategies for promoting single devices to the level of integrated circuits
is the key issue [17, 43–46]. In particular, for the realization of transistor circuits,
each component transistor is required to give sufficient signal amplification and to
be controlled by its own gate contact [17, 44–46]. Departing from this point, several approaches have been proposed to assembling logic circuits and nonvolatile
memory from carbon nanotube  and semiconductor nanowire [45–47] building
blocks. In the latter case, field-effect transistors (FETs) have been fabricated from
cross-point nanowire junctions  or core-multishell nanowire structures ,
and the crossing nanowire or metal contact evaporated on the outer shell, respectively, have been used as the local gate contacts. The important advantage of the
multishell-nanowire-based FETs lies in fact that they are by definition coaxially
gated transistors, and in this implement a strategy of “wrap-around gate” projected
for advancing conventional silicon transistors [1, 48, 49].
This chapter demonstrates the applicability of a “wrap-around gate” approach
to nanoscale thin film transistors (TFTs). We describe the synthesis and characterization of coaxially gated in-wire TFTs. These devices consist of a cadmium
chalcogenide thin film sandwiched between metal wire segments within a SiO2 tube.
The synthesis involves the above-described SSG deposition of SiO2 tubes on the
pore walls of an AAO membrane  and electroplating the composite nanowires
within the tubes . This approach is technologically simple and scalable with precise control over the diameter, segment lengths, and dielectric thickness. Two other
important advantages of the coaxially gated in-wire TFT structure are full encapsulation of the semiconductor segment, which prevents its oxidation, and possibility to
use metal gate electrodes, which are compatible with a variety of gate dielectrics .
In-wire TFTs were prepared as shown in Fig. 26.1, route 3. First, the Ag-backed
AAO membrane is subjected to deposition of SiO2 nanotubes on the pore walls
by repeating SiCl4 adsorption–hydrolysis cycles . The membrane is then used
as the cathode in an electrochemical cell to electroplate 3–5 μm long Au segments inside the SiO2 tubes. Semiconductor thin film segments are grown on the
tip of the Au wire using electrochemically induced CdS film growth [50, 51] or
cyclic voltametric CdSe deposition . Top Au segments 3–5 μm long are electroplated onto the cadmium chalcogenide films. Finally, the Au/CdS(Se)/Au@(SiO2 )n
(where n is the number of SSG cycles used for SiO2 –tube growth) nanowires
are released by dissolving the Ag backing and AAO membrane. Metal/CdS/metal
nanowires with different semiconductor segment lengths are prepared using 1 h
and 15 min deposition times. In the latter case Ag clusters were chemically
deposited prior to electrodeposition of the top metal segment in order to ensure
good electrical contact. These devices are referred to as Au/CdS/Au@(SiO2 )10 and
Au/CdS/AgAu@(SiO2 )14 , respectively.
An optical micrograph and TEM images of the in-wire TFT structures are shown
in Fig. 26.5a−c. The Au/CdS/Au junctions are clearly seen, and their thickness
Fig. 26.5 Optical micrograph (a) and TEM images (b, c) of Au/CdS/Au@(SiO2 )10 nanowires
prepared in AAO membranes with pore size 280±20 nm (a, b) and 70±10 nm (c). (d) Tapping
mode AFM image (585 × 585 nm, Z range 30.0o ) of CdS film prepared on an Au-coated glass
substrate using electrochemically induced deposition technique. Reprinted with permission from
. Copyright 2004 the American Chemical Society
Design and Assembly of High-Aspect-Ratio Silica-Encapsulated Nanostructures
can be roughly estimated at 100–200 nm for the wires prepared by using 1 h CdS
For the 15 min CdS deposition, TEM images show an approximate CdS film
thickness at 30–50 nm. An AFM image of a 31 nm thick CdS film prepared the
same way on a planar Au substrate shows densely packed 20–50 nm grains. An
XRD pattern of the planar CdS film (not shown) shows one CdS-related peak at
´ the position of which corresponds to the (111) reflection
2 = 26.65o (d = 3.34Å),
´ or the (002) reflection of the hexagonal
of the cubic zinc blend structure (d = 3.36 Å)
´ However, the absence of other strong peaks from
wurzite structure (d = 3.36Å).
(100) and (101) planes of the hexagonal phase indicates that CdS crystallizes mainly
in the cubic phase, in contrast to the hexagonal phase formed on ITO and SnO2
substrates . The average crystal size estimated from the X-ray line widths is
39.6 nm, which is consistent with the AFM data.
The thickness of the SiO2 tubes that encapsulate the nanowires is uniform along
the wire length and ranges from 12 to 14 nm for 10 SSG cycles (Fig. 26.5b) and
from 16 to 18 nm for 14 SSG cycles. The flexibility of these shells allows them to
precisely follow the shape of Au/CdS/Au junctions (Fig. 26.5b) thus enabling good
adhesion of the gate dielectric to the semiconductor film.
The nanowires were aligned as shown in Fig. 26.6a for electrical measurements.
IDS −VDS characteristics of Au/CdS/Au@(SiO2 )10 and Au/CdS/AgAu@(SiO2 )14
devices are shown in Fig. 26.6b, c. At zero gate bias (VGS = 0), turn-on potentials
are −0.6 and −0.2 V, respectively, which is in reasonable agreement with the differences between the electron affinity of CdS (∼4.5 eV) and the Au (∼5.2 eV) and
Ag (∼4.7 eV) work functions, respectively. The Au/CdS/AgAu@(SiO2 )14 devices
show a zero gate bias DS resistivity 55 times lower than Au/CdS/Au@(SiO2 )10 ,
which may be attributed to better CdS/Ag electrical contact due to the formation
of Ag−S bonds, and possibly to fewer grain boundaries in the thinner CdS film.
However, the metal/semiconductor contacts of the in-wire TFTs are still much more
resistive than those of planar TFTs [52, 53]. This implies a stronger effect of the
contact resistance on the nanowire device properties. Therefore, all characteristics
described below result from a field effect on both the CdS channel and Au(Ag)/CdS
The IDS −VDS characteristics of both devices clearly show a field effect, which
is more pronounced at negative drain voltage (Fig. 26.6b, c). At VDS = −2 V, the
Au/CdS/Au@(SiO2 )10 devices have an ON/OFF current ratio of 103 , a threshold
voltage of 2.4 V, and a sub-threshold slope of 2.2 V per decade (Fig. 26.6d, gr. 1, 3).
The Au/CdS/AgAu@(SiO2 )14 devices show similar parameters at VDS = −0.2 V
and a gate sweep from 0 to 10 V. While the in-wire TFTs can operate at relatively low drain voltages, the above parameters are superior to those found with
planar CdS  and nanocrystal-derived CdSe [53a]. TFTs in the gate voltage
range from ±9 to10V. The lower VT and a threefold decrease in the sub-threshold
slope (S) relative to planar nanocrystal-derived CdSe TFTs (S 7−10 V per decade
[53a]) may result from the thinner dielectric layer and coaxial gating. A similar
tendency was predicted for planar double-gated versus conventional FETs .
Fig. 26.6 (a) An optical micrograph and schematic presentation of the test structure and
Au/CdS/Au@(SiO2 )10 nanowire aligned for measuring the electrical properties. Letters S, D, and
G indicate source, drain, and gate electrodes, respectively; (b, c) IDS −VDS characteristics of in-wire
TFTs for different values of gate voltage (VGS ): (b) Au/CdS/Au@(SiO2 )10 //Au (CdS deposition
for 1 h); (c) Au/CdS/AgAu@(SiO2 )14 //Au (CdS deposition for 15 min). Gate leakage currents
were√in the range of 10–14 –10–12 A.; (d) IDS −VGS characteristics of in-wire TFTs: Log IDS (1, 1∗ )
and IDS (3) for Au/CdS/Au@(SiO2 )10 //Au at VDS = −2 V for a gate sweep from −9 to 9 V (1)
and vice versa (1∗ ); (2) Log IDS for Au/CdSe/Au@(SiO2 )14 //Au at VDS = 5 V for a gate sweep
from 0 to 8 V. All measurements were performed in air at ambient temperature with a HP 4156B
Precision Semiconductor Parameter Analyzer. Compliance current was set up at 1 nA. The TFTs
were prepared using commercial AAO membranes with pore size 280 ± 20 nm. Reprinted with
permission from . Copyright 2004 the American Chemical Society
On the other hand, the channel mobility of the in-wire TFTs is approximately
5 ± 2 × 10−5 cm2 V−1 s−1 . This is 4–6 orders of magnitude lower than that
found for TFTs with several micron long channels of planar nanocrystal-derived
and vapor-deposited CdSe and CdS [13, 14]. To a certain extent, this decrease may
be caused by the significant reduction of the channel length in the in-wire TFTs. The
field-dependent mobility decrease is a predicted consequence of FET channel scaling [48, 54]. However, high Schottky contact resistance is most likely responsible
for the low apparent mobility values. We believe that much higher mobility values
can be achieved by further improving the metal/semiconductor interfaces and grain
Design and Assembly of High-Aspect-Ratio Silica-Encapsulated Nanostructures
structure of the semiconductor segment, as well as by using metal contacts with
lower work function. Au/CdSe/Au@(SiO2 )14 TFTs show poorer performance with
an ON/OFF current ratio about 10 (Fig. 26.6d, gr. 2). This is consistent with observation by other groups  that planar CdSe TFTs fabricated without annealing
exhibit very weak, if any, field effect.
Log (IDS )−VGS graphs with a gate sweep from −9 to 9 V and vice versa
(Fig. 26.3d, gr. 1, 1∗ ) show CCW hysteresis contrary to the CW one observed with
planar CdSe TFTs . The origin of the hysteresis is not currently understood but
may be tentatively ascribed to trap states at the semiconductor/SiO2 interface .
However, the chemical nature of the traps in our wet-assembled in-wire devices may
differ from that in the thermally evaporated or annealed planar TFTs. Also a field
effect on the Au/CdS contact properties may cause the CCW hysteresis. Oxidation
of the planar TFTs [53a] is a less likely source of trap states in this case because the
in-wire TFTs are encapsulated by SiO2 .
The surface sol–gel method is a simple way to prepare robust and flexible silica
nanotubes. The thickness and porosity of the tubes can be precisely controlled by
varying the composition of the precursor solution and the number of adsorption–
hydrolysis cycles. The thickness of the SiO2 layer deposited in each cycle,
which always exceeds that of a monomolecular layer, can be explained assuming
occlusion of water present as a surface layer. Free-standing SiO2 nanotubes with
2–30 nm walls, which are smooth and uniform along their length, were grown and
The SSG thin film deposition technique is well developed for other classes of
materials, including metal oxides, chalcogenides, and phosphates. When performed
in porous templates, as we have demonstrated here for SiO2 , the SSG method should
offer a route to concentric multicomponent structures with well-controlled layer
thickness and, presumably, tunable electrical and optical properties. The good control in film thickness that is obtained by SSG suggests that it should also be possible
to precisely adjust the internal diameter of the AAO pores, and hence the diameter
of nanowire replicas.
Electroplating metals inside the silica-coated pores of an AAO membrane is
an easy route to nanoscale insulated metal interconnects of high quality. The hard
breakdown field obtained for insulating SiO2 -nanotube coating on gold nanowires
is only slightly lower than that of SiO2 dielectric used in CMOS integrated circuits,
and this is a surprising result given the fact that a wet chemical deposition method
Coaxially gated in-wire thin film transistors can be made by using a combination of the templated SSG technique and electrochemical deposition of composite
nanowires. The CdS-based TFTs can operate at drain voltages lower than 1 V
and show better ON/OFF current ratio, threshold voltage, and sub-threshold slope
than chemically similar planar TFTs. While the devices described here were not
optimized for performance, one might expect significant improvements by using
strategies that have been developed or predicted for conventional FETs and TFTs
[48, 52, 54]. The control of dimensions afforded by the template synthesis should
make it possible to reduce the gate dielectric thickness, channel length, and diameter
of the semiconductor body (see, e.g., Fig. 26.5c). The latter would extend the gate
effect across the body region  and might also result in the formation of singlecrystal semiconductor segments . The SSG technique can be easily extended to
other metal oxides that will allow substitution of higher k dielectrics, such as zirconium, titanium, and tantalum oxides for SiO2 . Finally, thermal annealing of the
semiconductor segment prior to top electrode deposition is expected to improve the
performance of the CdSe-based devices.
Acknowledgments I am grateful to Tom Mallouk for his deep interest and support of this work. I
thank T.N. Jackson, T.S. Mayer, B. Kelley, and C.S. Kuo, who contributed to the work described in
this chapter. This work was supported by the DARPA/ONR Moletronics program and by National
Science Foundation grant CHE-0095394.
1. Vogel, E.: Technology and Metrology of New Electronic Materials and Devices. Nat.
Nanotechnol. 2, 25 (2007).
2. Chau, R., Doyle, B., Datta, S., Kavalieros, J., Zhang, K.: Integrated Nanoelectronics for the
Future. Nat. Mater. 6, 810–812 (2007).
3. Law, M., Goldberger, J., Yang, P. D.: Semiconductor Nanowires and Nanotubes. Annu. Rev.
Mater. Res. 34, 83–122 (2004).
4. (a) Dresselhaus, M. S., Dresselhaus, G., Jorio, A.: Unusual Properties and Structure of Carbon
Nanotubes. Annu. Rev. Mater. Res. 34, 247–278 (2004); (b) Chen, J., Klinke, C., Afzali, A.,
Avouris, P.: Self-Aligned Carbon Nanotube Transistors with Charge Transfer Doping. Appl.
Phys. Lett. 86, 123108 (2005).
5. Kovtyukhova, N. I., Mallouk, T. E.: Nanowires as Building Blocks for Self-Assembling Logic
and Memory Circuits. Chem. Eur. J. 8, 4355–4363 (2002).
6. Huynh, W., Dittmer, J., Alivisatos, A. P.: Hybrid Nanorod-Polymer Solar Cells. Science 295,
7. Tian, B., Zheng, X., Kempa, T. J., Fang, Y., Yu, N., Yu, G., Huang, J., Lieber, C. M.: Coaxial
Silicon Nanowires as Solar Cells and Nanoelectronic Power Sources. Nature 449, 885–889
8. Bae, C., Yoo, H., Kim, S., Lee, K., Kim, J., Sung, M. M., Shin, H.: Template-Directed
Synthesis of Oxide Nanotubes: Fabrication, Characterization and Applications. Chem. Mater.
20, 756–767 (2008).
9. Katz, E., Willner, I.: Biomolecule-Functionalized Carbon Nanotubes: Applications in
Nanobioelectronics. Chem. Phys. Chem. 5, 1084 (2004).
10. Heath, J. R.: Label-Free Nanowire and Nanotube Biomolecular Sensors for In Vitro
Diagnostics of Cancer and Other Diseases. In: Mirkin, C., Niemeyer, C. M. (eds.)
Nanobiotechnology II: Concepts, Applications, and Perspectives, Wiley, New York (2007).
11. Chan, C. K., Peng, H., Liu, G., McIlwrath, K., Zhang, X. F., Huggins, R. A., Cui, Y.: HighPerformance Lithium Battery Anodes Using Silicon Nanowires. Nat. Nanotechnol. 3, 31–35
12. Paxton, W. F., Kistler, K. C., Olmeda, C. C., Sen, A., St. Angelo, S. K., Cao, Y., Mallouk,
T., Lammert, P. E., Crespi, V. H.: Catalytic Nanomotors: Autonomous Movement of Striped
Nanorods. J. Am. Chem. Soc. 126, 13424 (2004)
Design and Assembly of High-Aspect-Ratio Silica-Encapsulated Nanostructures
13. (a) Fournier-Bidoz, S., Arsenault, A. C., Manners, I., Ozin, G. A.: Synthetic Self-Propelled
Nanorotors. Chem. Commun. 441 (2005); (b) Ozin, G. A., Manners, I., Fournier-Bidoz, S.,
Arsenault, A.: Dream Nanomachines. Adv. Mater. 17, 3011 (2005).
14. Kovtyukhova, N.: Toward Understanding of the Propulsion Mechanism of Rod-Shaped
Nanoparticles That Catalyze Gas-Generating Reactions. J. Phys. Chem. C 112, 6049 (2008).
15. Burghard, M.: A Freight Train of Nanotubes for Cargo Transport on the Nanoscale. Angew.
Chem. Int. Ed. 47, 8565–8566 (2008).
16. Sundararajan, S., Lammert, P. E., Zudans, A. W., Crespi, V. H., Sen, A.: Catalytic Motors for
Transport of Colloidal Cargo. Nano Lett. 8, 1271 (2008).
17. Tseng, G., Ellenbogen, J.: Toward Nanocomputers. Science 294, 1293 (2001).
18. Goldstein, S. C., Budiu, M.: In: Proc. 28th Annu. Int. Symp. Computer Architecture 2001,
Göteborg, Sweden, p. 178, ACM Press, New York (2001).
19. Sheriff, B. A., Wang, D., Heath, J. R., Kurtin, J. N.: Complementary Symmetry Nanowire
Logic Circuits: Experimental Demonstrations and In Silico Optimizations. ACS Nano 2,
20. Green, J. E., Choi, J. W., Boukai, A., Bunimovich, Y., Johnston-Halperin, E., DeIonno, E.,
Luo, Y., Sheriff, B. A., Xu, K., Shin, Y. S., Heatrh J. R.: A 160-Kilobit Molecular Electronic
Memory Patterned at 10(11) Bits Per Square Centimetre. Nature 445, 414–417 (2007).
21. Meyyappan, M. (ed.): Carbon Nanotubes: Science and Applications, CRS Press, Boca Raton
22. (a) Martin, B. R., Dermody, D. J., Reiss, B. D., Fang, M., Lyon, L. A., Natan, M. J., Mallouk,
T. E.: Orthogonal Self-Assembly on Colloidal Gold-Platinum Nanorods. Adv. Mater. 11, 1021
(1999); (b) Mbindyo, J. K. N., Reiss, B. D., Martin, B. R., Keating, C. D., Natan, M. J.,
Mallouk, T. E.: DNA-Directed Assembly of Gold Nanowires on Complementary Surfaces.
Adv. Mater. 13, 249 (2001); (c) Reiss, B. D., Mbindyo, J. N. K., Martin, B. R., Nicewarner,
S. R., Mallouk, T. E., Natan, M. J., Keating, C. D.: DNA-Directed Assembly of Anisotropic
Nanoparticles on Lithographically Defined Surfaces and in Solution. Mater. Res. Soc. Symp.
Proc. 635, C6.2.1 (2001).
23. (a) Kovtyukhova, N. I., Mallouk, T. E.: Nanowire p-n Heterojunction Diodes Made by
Templated Assembly of Multilayer Carbon-Nanotube/Polymer/Semiconductor-Particle Shells
Around Metal Nanowires. Adv. Mater. 17, 187–192 (2005); (b) Kovtyukhova, N. I., Martin,
B. R., Mbindyo, J. K. N., Smith, P. A., Razavi, B., Mayer, T. S., Mallouk, T. E.: Layer by
Layer Assembly of Rectifying Junctions in and on Metal Nanowires. J. Phys. Chem. B 105,
8762–8769 (2001); (c) Kovtyukhova, N. I., Martin, B. R., Mbindyo, J. K. N., Mallouk, T. E.,
Cabassi, M., Mayer, T. S.: Layer by Layer Self-Assembly Strategy for Template Synthesis of
Nanoscale Devices. Mater. Sci. Eng. C 19, 255 (2002).
24. Kovtyukhova, N. I., Mallouk, T. E., Mayer, T. S.: Templated Surface Sol-Gel Synthesis of
SiO2 Nanotubes and SiO2 -Insulated Metal Nanowires. Adv. Mater. 15, 780 (2003).
25. Kovtyukhova, N. I., Kelley, B. K., Mallouk, T. E.: Coaxially Gated In-Wire Thin Film
Transistors. J. Am. Chem. Soc. 126, 12738 (2004).
26. Park, S., Chung, S. W., Mirkin, C: Hybrid Organic–Inorganic, Rod-Shaped Nanoresistors and
Diodes. J. Am. Chem. Soc. 126, 11772–11773 (2004).
27. (a) Al-Mawlawi, D., Liu, C. Z., Moskovits, M.: Nanowires Formed in Anodic Oxide
Nanotemplates. J. Mater. Res. 9, 1014 (1994); (b) Nishizava, M., Menon, V. P., Martin, C. R.:
Metal Nanotubule Membranes with Electrochemically Switchable Ion-Transport Selectivity.
Science 268, 700 (1995).
28. (a) Colvin, V., Schlamp, M., Alivisatos, A. P.: Light-Emitting Diodes Made from
Cadmium Selenide Nanocrystals and a Semiconducting Polymer. Nature 370, 354 (1994);
(b) Cassagneau, T., Mallouk, T. E., Fendler, J. H.: Layer-by-Layer Assembly of Thin-Film
Zener Diodes from Conducting Polymers and CdSe Nanoparticles. J. Am. Chem. Soc. 120,
7848 (1998); (c) Gao, M., Richter, B., Kirstein, S., Mohwald, H.: Electroluminescence
Studies on Self-Assembled Films of PPV and CdSe Nanoparticles. J. Phys. Chem. 102,
4096 (1998); (d) Kaschak, D., Lean, J., Waraksa, C., Saupe, G., Usami, H., Mallouk, T.:
Photoinduced Energy and Electron Transfer Reactions in Lamellar Polyanion/Polycation Thin
Films: Toward an Inorganic “Leaf”. J. Am. Chem. Soc. 121, 3435 (1999); (e) Feldheim,
D., Grabar, K., Natan, M., Mallouk, T.: Electron Transfer in Self-Assembled Inorganic
Polyelectrolyte/Metal Nanoparticle Heterostructures. J. Am. Chem. Soc. 118, 7640 (1996).
(a) Ichinose, I., Senzu, H., Kunitake, T.: A Surface Sol-Gel Process of TiO2 and Other Metal
Oxide Films with Molecular Precision. Chem. Mater. 9, 1296 (1997); (b) Fang, M., Kim,
C. H., Martin, B. R., Mallouk, T. E.: Surface Sol–Gel Synthesis of Ultrathin Titanium and
Tantalum Oxide Films. J. Nanoparticle Res. 1, 43–49 (1999).
Kovtyukhova, N. I., Buzaneva, E. V., Waraksa, C. C., Martin, B., Mallouk, T. E.: Surface
Sol-Gel Synthesis of Ultrathin Semiconductor Films. Chem. Mater. 12, 383 (2000).
Pena, D., Mbindyo, J., Carado, A., Mallouk, T., Keating, C., Razavi, B., Mayer, T.: Template
Growth of Photoconductive Metal-CdSe-Metal Nanowires. J. Phys. Chem. B 106, 7458
Cao, Y., Kovalev, A. E., Kim, J., Mayer, T. S., Mallouk, T. E.: Electrical Transport and
Chemical Sensing Properties of Individual Conducting Polymer Nanowires. Nano Lett., 8,
Nalwa, H. S. (ed.): Handbook of Low and High Dielectric Constant Materials and Their
Applications V1, Academic Press, New York (1999).
Riley, G.: The race to replace copper. In: Advanced Packaging, E-Newsletter, 20 February
(a) Mitchell, D. T., Lee, S. B., Trofin, L., Li, N., Nevanen, T. K., Soderlund, H., Martin,
C. R.: Smart Nanotubes for Bioseparations and Biocatalysis. J. Am. Chem. Soc. 124, 11864
(2002); (b) Lakshmi, B. B., Dorhout, P. K., Martin, C. R.: Sol-Gel Template Synthesis of
Semiconductor Nanostructures. Chem. Mater. 9, 857 (1997); (c) Lakshmi, B. B., Patrissi,
C. J., Martin, C. R.: Sol-Gel Template Synthesis of Semiconductor Oxide Micro- and
Nanostructures. Chem. Mater. 9, 2544 (1997).
Zhang, M., Bando, Y., Wada, K.: Silicon Dioxide Nanotubes Prepared by Anodic Alumina as
Templates. J. Mater. Res. 15, 387 (2000).
(a) Iler, R. K.: Multilayers of Colloidal Particles. J. Colloid Interface Sci. 21, 569 (1966);
(b) Colvin, V. L., Golstein, A. N., Alivisatos, A. P.: Semiconductor Nanocrystals Covalently
Bound to Metal Surfaces with Self-Assembled Monolayers. J. Am. Chem. Soc. 114, 5221
(1992); (c) Fendler, J.: Self-Assembled Nanostructured Materials. Chem. Mater. 8, 1616
(1996); (d) Mallouk, T. E., Kim, H.-N., Ollivier, P. J., Keller, S. W.: Ultrathin Films Based on
Layered Materials. In: Alberti, G., Bein, T. (eds.) Comprehensive Supramolecular Chemistry
V7, p. 189, Elsevier Science, Oxford (1996).
Kleinfeld, E. R., Ferguson, G. S.: Healing of Defects in the Stepwise Formation of
Polymer/Silicate Multilayer Films. Chem. Mater. 8, 1575 (1996).
Nicolau, Y. F., Menard, J. C.: Solution Growth of Zinc Sulfide, Cadmium Sulfide and Zinc
Cadmium Sulfide Thin Films by the Successive Ionic-Layer Adsorption and Reaction Process;
Growth Mechanism. J. Crystal Growth 92, 128 (1988).
Parfitt, G. D., Rochester C. H. (eds.): Adsorption from Solution at the Solid/Liquid Interface,
Academic Press, London (1983).
Weas, R. C. (ed.): Handbook of Chemistry and Physics, 68th Ed., CRS Press, Boca Raton
Jin, C., Luttmer, J. D, Smith, D. M., Ramos, T. A.: Nanoporous Silica as an Ultralow-k
Dielectrics. MRS Bull. 22, 10, 39 (1997).
Zhong, Z., Wang, D., Cui, Y., Bockrath, M. W., Lieber, C. M.: Nanowire Crossbar Arrays as
Address Decoders for Integrated Nanosystems. Science 302, 1377 (2003).
Bachtold, A., Hadley, P., Nakanishi, T., Dekker, C.: Logic Circuits with Carbon Nanotube
Transistors. Science 294, 1317 (2001).
Huang, Y., Duan, X., Cui, Y., Lauhon, L., Kim, K., Lieber, C. M.: Logic Gates and
Computation from Assembled Nanowire Building Blocks. Science 294, 1313 (2001).
Lauhon, L., Gudiksen, M., Wang, D., Lieber, C. M.: Epitaxial Core-Shell and Core-Multishell
Nanowire Heterostructures. Nature 420, 57 (2002).
Design and Assembly of High-Aspect-Ratio Silica-Encapsulated Nanostructures
47. Duan, H., Huang, Y., Lieber, C. M.: Nonvolatile Memory and Programmable Logic from
Molecule-Gated Nanowires. Nano Lett. 2, 487 (2002).
48. Solomon, P. M.: Device Innovation and Material Challenges at the Limits of CMOS
Technology. Annu. Rev. Mater. Sci. 30, 681 (2000).
49. Leobandung, E., Gu, J., Guo, L., Chou, S.: Wire-Channel and Wrap-Around-Gate Metal–
Oxide–Semiconductor Field-Effect Transistors with a Significant Reduction of Short Channel
Effects. J. Vac. Sci. Technol. B 15, 2791 (1997).
50. Yamaguchi, K., Yoshida, T., Sugiura, T., Minoura, H.: A Novel Approach for CdS ThinFilm Deposition: Electrochemically Induced Atom-by-Atom Growth of CdS Thin Films from
Acidic Chemical Bath. J. Phys. Chem. B 102, 9677 (1998).
51. Xu, D., Xu, Y., Chen, D., Guo, G., Gui, L., Tang, Y.: Preparation of CdS Single-Crystal
Nanowires by Electrochemically Induced Deposition. Adv. Mater. 12, 520 (2000).
52. Weimer, P. K.: The TFT – A New Thin-Film Transistor. Proc. IRE 1462 (1962).
53. (a) Ridley, B., Nivi, B., Jacobson, J.: All-Inorganic Field Effect Transistors Fabricated by
Printing. Science 286, 746 (1999); (b) Reita, C.: Theory for field-effect mobility enhancement
in multilayer structure thin-film transistors. Inf. Display 2, 10 (1993).
54. (a) Sze, S. M.: Physics of Semiconductor Devices, Wiley, New York (1981); (b) Ando, T.,
Fowler, A., Stern, F.: Electronic Properties of Two-Dimensional Systems. Rev. Mod. Phys.
54, 437 (1982).
Physicochemical Properties and
Biocompatibility of Polymer/Carbon
Yu.I. Sementsov, G. P. Prikhod’ko, A.V. Melezhik,
T.A. Aleksyeyeva, and M.T. Kartel
Abstract Due to the unique structure and combination of extremely high durability, electrical and calorific conductivities, carbon nanotubes (CNTs) are prospective
fillers for polymer materials. The reinforcement of polymer by developed set-like
form of CNT provides an increase in mechanical, electrical, and thermophysical
properties, chemical stability, and biocompatibility of nanocomposites. The manufacture of CNT and polymers (polypropylene, Teflon-4, and elastomers on the base
of butadiene–nitrile and fluorinated rubbers) filled with nanotubes and nanofibers
of various contents is described. The CNT and the nanocomposites are characterized in detail by structural and physicochemical methods. It is shown that not only
bulk characteristics but also surface properties of filled polymers are changed and
this explains better the biocompatibility of nanocomposites, which is observed in in
Development of medicine, especially for rehabilitation, is connected with searching
for new materials to produce and substitute an organism’s parts damaged due to
illness. Presently there are vast possibilities to create artificial prosthetic appliances
of practically any organ.
So the problem is to develop (to create) new materials which would have
biomechanical characteristics similar to natural ones. Due to the unique structure and combination of high durability, electro- and thermoconductivity, carbon
nanotubes are prospective fillings for creation of new composite materials . In this
work, structural features, physical and mechanical characteristics were studied of
nanocomposites on the base of polytetrafluoroethylene (PTFE), isotactic polypropylene (PP), butadiene–nitrile, and fluorinated rubbers with CNT as filler. Also some
biocompatibility properties were studied in experiments in vivo.
M.T. Kartel (B)
O.O. Chuiko Institute of Surface Chemistry of the National Academy of Sciences of Ukraine,
General Naumov St. 17, Kyiv 03164, Ukraine
A.P. Shpak, P.P. Gorbyk (eds.), Nanomaterials and Supramolecular Structures,
DOI 10.1007/978-90-481-2309-4_27, C Springer Science+Business Media B.V. 2009